Citation:Wallah, S.E. and Rangan, B.V. 2006. Low-Calcium fly ash-based geopolymer concrete: Long-term properties.Curtin University of Technology.
Additional Information:For further information, please contact: Professor B. Vijaya Rangan BE PhD FIE Aust
FACI, CPEng, Emeritus Professor of Civil Engineering, Faculty of Engineering, Curtin
University of Technology, Perth, WA 6845, Australia; Telephone: 61 8 9266 1376, Email:
The attached document may provide the author's accepted version of a published work.See Citation for details of the published work.
LOW-CALCIUM FLY ASH-BASED GEOPOLYMER CONCRETE: LONG-TERM
S. E. Wallah and B. V. Rangan
Research Report GC 2 Faculty of Engineering
Curtin University of Technology Perth, Australia
From 2001, we have conducted some important research on the development, manufacture, behaviour, and applications of Low-Calcium Fly Ash-Based Geopolymer Concrete. This concrete uses no Portland cement; instead, we use the low-calcium fly ash from a local coal burning power station as a source material to make the binder necessary to manufacture concrete.
Concrete usage around the globe is second only to water. An important ingredient in the conventional concrete is the Portland cement. The production of one ton of cement emits approximately one ton of carbon dioxide to the atmosphere. Moreover, cement production is not only highly energy-intensive, next to steel and aluminium, but also consumes significant amount of natural resources. In order to meet infrastructure developments, the usage of concrete is on the increase. Do we build additional cement plants to meet this increase in demand for concrete, or find alternative binders to make concrete?
On the other hand, already huge volumes of fly ash are generated around the world; most of the fly ash is not effectively used, and a large part of it is disposed in landfills. As the need for power increases, the volume of fly ash would increase.
Both the above issues are addressed in our work. We have covered significant area in our work, and developed the know-how to manufacture low-calcium fly ash-based geopolymer concrete. Our research has already been published in more than 30 technical papers in various international venues.
This Research Report describes the long-term properties of low-calcium fly ash-based geopolymer concrete. Earlier, the Research Report GC1 presented the development, the mixture proportions, and the short-term properties of low-calcium fly ash-based geopolymer concrete. A subsequent Research Report GC3 covers the behaviour and strength of reinforced geopolymer concrete structural beams and columns.
Heat-cured low-calcium fly ash-based geopolymer concrete has excellent compressive strength, suffers very little drying shrinkage and low creep, excellent resistance to sulfate attack, and good acid resistance. It can be used in many infrastructure applications. One ton of low-calcium fly ash can be utilised to produce about 2.5 cubic metres of high quality geopolymer concrete, and the bulk price of chemicals needed to manufacture this concrete is cheaper than the bulk price of one ton of Portland cement. Given the fact that fly ash is considered as a waste material, the low-calcium fly ash-based geopolymer concrete is, therefore, cheaper than the Portland cement concrete. The special properties of geopolymer concrete can further enhance the economic benefits. Moreover, reduction of one ton of carbon dioxide yields one carbon credit and, the monetary value of that one credit is approximately 20 Euros. This carbon credit significantly adds to the economy offered by the geopolymer concrete. In all, there is so much to be gained by using geopolymer concrete.
We are happy to participate and assist the industries to take the geopolymer concrete technology to the communities in infrastructure applications. We passionately believe that our work is a small step towards a broad vision to serve the communities for a better future.
For further information, please contact: Professor B. Vijaya Rangan BE PhD FIE Aust FACI, CPEng, Emeritus Professor of Civil Engineering, Faculty of Engineering, Curtin University of Technology, Perth, WA 6845, Australia; Telephone: 61 8 9266 1376, Email: V.Rangan@curtin.edu.au
The authors are grateful to Emeritus Professor Joseph Davidovits, Director, Geopolymer Institute, Saint-Quentin, France, and to Dr Terry Gourley, Rocla Australia for their advice and encouragement during the conduct of the research.
An Australian Development Scholarship supported the first author. The authors are grateful to Mr. Djwantoro Hardjito and Mr. Dody Sumajouw, the other members of the research team, for their contributions.
The experimental work was carried out in the laboratories of the Faculty of Engineering at Curtin University of Technology. The authors are grateful to the
support and assistance provided by the team of talented and dedicated technical staff comprising Mr. Roy Lewis, Mr. John Murray, Mr. Dave Edwards, Mr. Rob Cutter, and Mr. Mike Ellis.
TABLE OF CONTENTS
TABLE OF CONTENTS i LIST OF FIGURES iv LIST OF TABLES vii CHAPTER I: INTRODUCTION 1 1.1. Background 1
1.2. Objectives 2 1.3. Scope of the Work 2 1.4. Organisation of Report 3 CHAPTER 2: LITERATURE REVIEW 4 2.1. Introduction 4
2.2. Geopolymers 4 2.2.1. Terminology and Chemistry 4 2.2.2. Source Materials and Alkaline Liquids 6 2.2.3. Fields of Applications 8 2.2.4. Properties of Geopolymers 10
CHAPTER 3: EXPERIMENTAL WORK 12 3.1. Introduction 12 3.2. Materials 12 3.2.1. Fly Ash 12 3.2.2. Aggregates 14 3.2.3. Alkaline Liquid 15 3.2.4. Super plasticiser 15 3.3. Mixture Proportions 15 3.4. Manufacture of Test Specimens 17 3.4.1. Preparation of Liquids 17 3.4.2. Manufacture of Fresh Concrete and Casting 17 3.4.3. Manufacture of Fresh Mortar and Casting 19
3.5. Curing Of Test Specimens 20 3.6. Compressive Strength Test 22 3.7. Creep Test 22 3.7.1. Test Specimens 22 3.7.2. Test Parameters 23 3.7.3. Test Procedure 23 126.96.36.199. Strain Measuring Device and Reference Gauge Points 23 188.8.131.52 Test Set up and Measurement 24
3.8. Drying Shrinkage Test 26 3.8.1. Test Specimens 26 3.8.2. Test parameters 27 3.8.3. Test Procedure 27
3.9. Sulfate Resistance Test 28 3.9.1. Test Specimens 28 3.9.2. Test parameters 29 3.9.3. Test Procedure 29 184.108.40.206. Sulfate Solution 29 220.127.116.11. Change in Compressive Strength 30 18.104.22.168. Change in Mass 30 22.214.171.124. Change in Length 31 3.10. Acid Resistance Test 31 3.10.1. Tests of Geopolymer Concrete 32 3.10.2. Tests of Geopolymer Mortar 32
CHAPTER 4: PRESENTATION AND DISCUSSION OF EXPERIMENTAL RESULTS
4.1. Introduction 34
4.2. Compressive Strength and Unit Weight 34 4.2.1 Mean compressive strength and unit-weight 34 4.2.2. Effect of age on compressive strength and unit weight 35 4.2.3. Compressive strength of specimens cured at ambient conditions 37 4.3. Creep 38 4.3.1. Test results 38 4.3.2. Effect of Compressive Strength 46 4.3.3 Correlation of Test Results with Predictions by Australian Standard AS3600
4.4. Drying Shrinkage 52 4.4.1. Drying shrinkage of heat-cured geopolymer concrete specimens 52 4.4.2. Drying shrinkage of heat-cured specimens versus ambient-cured specimens
4.4.3 Correlation of test results with prediction by Australian Standard AS3600
4.5. Sulfate Resistance 59 4.5.1. Visual appearance 59 4.5.2. Change in Length 60 4.5.3. Change in mass 61 4.5.4. Change in compressive strength 62 4.6. Acid Resistance 66 4.6.1. Visual appearance 67 4.6.2. Test on concrete specimens 68 4.6.3. Tests on mortar specimens 73 CHAPTER 5: CONCLUSIONS 75 5.1. Introduction 75 5.2. Conclusions 77
REFERENCES 80 APPENDIX A 86 APPENDIX B 91
LIST OF FIGURES
Figure 2.1 Chemical structures of polysialates 5 Figure 3.1 Particle Size Distribution of Batch-1 Fly Ash 13 Figure 3.2 Particle Size Distribution of Batch-2 Fly Ash 14
Figure 3.3 Particle Size Distribution of Batch-3 Fly Ash 14 Figure 3.4 Fresh Geopolymer Concrete 18 Figure 3.5 Compaction of Concrete Specimens 18 Figure 3.6 Measurement of slump 19 Figure 3.7 Fresh Geopolymer Mortar 19 Figure 3.8 Compaction of Mortar Specimens 20 Figure 3.9 Dry Curing 21 Figure 3.10 Steam Curing 21 Figure 3.11 Creep Test Specimens 22 Figure 3.12 Location of Demec Gauge Points on Test Cylinders 24 Figure 3.13 Creep Test Set-up 25 Figure 3.14 Creep Test 25 Figure 3.15 Specimens for Drying Shrinkage Test 26 Figure 3.16 Horizontal length comparator with a specimen 28 Figure 3.17 Specimens for Sulfate Resistance Test 28 Figure 3.18 Specimens Soaked in Sodium Sulfate Solution 30 Figure 4.1 Change in compressive strength with age 36 Figure 4.2 Change in unit weight with age 36 Figure 4.3 Compressive strength of concrete cured at ambient condition 38 Figure 4.4 Total and drying shrinkage strain for 1CR 40 Figure 4.5 Total and drying shrinkage strain for 2CR 40 Figure 4.6 Total and drying shrinkage strain for 3CR 40 Figure 4.7 Total and drying shrinkage strain for 4CR 41 Figure 4.8 Creep strain for 1CR 41 Figure 4.9 Creep strain for 2CR 42 Figure 4.10 Creep strain for 3CR 42 Figure 4.11 Creep strain for 4CR 42
Figure 4.12 Creep coefficient for 1CR 43 Figure 4.13 Creep coefficient for 2CR 43 Figure 4.14 Creep coefficient for 3CR 44 Figure 4.15 Creep coefficient for 4CR 44 Figure 4.16 Specific creep for 1CR 45 Figure 4.17 Specific creep for 2CR 45 Figure 4.18 Specific creep for 3CR 45 Figure 4.19 Specific creep for 4CR
Figure 4.20 Creep of concrete of different strength 47 Figure 4.21 Maturity coefficient k3 (Gilbert 2002) 48 Figure 4.22 Correlation of Test and Predicted Creep strains: Specimen 1CR 50 Figure 4.23 Correlation of Test and Predicted Creep strains: Specimen 2CR 50 Figure 4.24 Correlation of Test and Predicted Creep strains: Specimen 3CR 51 Figure 4.25 Correlation of Test and Predicted Creep strains: Specimen 4CR 51 Figure 4.26 Drying shrinkage of heat-cured Mixture-1 specimens 54 Figure 4.27 Drying shrinkage of heat-cured Mixture-2 specimens 54 Figure 4.28 Drying shrinkage of heat-cured and ambient-cured specimens 55 Figure 4.29 Comparison of test and predicted results for 1DS 57 Figure 4.30 Comparison of test and predicted results for 2DS 57 Figure 4.31 Comparison of test and predicted results for 3DS 58 Figure 4.32 Comparison of test and predicted results for 4DS 58 Figure 4.33 Comparison of test and predicted results for 5DS 59 Figure 4.34 Visual appearance of test specimens after exposure 60 Figure 4.35 Change in length of specimens exposed to sodium sulfate solution
Figure 4.36 Change in mass of specimens soaked in sodium sulfate solution and water
Figure 4.37 Compressive strength after 4 weeks of exposure 62 Figure 4.38 Compressive strength after 8 weeks of exposure 63 Figure 4.39 Compressive strength after 12 weeks of exposure 63 Figure 4.40 Compressive strength after 24 weeks of exposure 63 Figure 4.41 Compressive strength after 52 weeks of exposure 64 Figure 4.42 Visual appearance after one year of exposure in sulfuric acid solution
Figure 4.43 Visual appearance of mortar specimens after one year exposure in sulfuric acid solution
Figure 4.44 Damage to test cylinders exposed to 2% sulfuric acid solution 68 Figure 4.45 Change in mass of concrete exposed to sulfuric acid solution 69 Figure 4.46 Compressive strength of geopolymer concrete exposed to 2% sulfuric acid solution
Figure 4.47 Compressive strength of geopolymer concrete exposed to 1% sulfuric acid solution
Figure 4.48 Compressive strength of geopolymer concrete exposed to 0.5% sulfuric acid solution
Figure 4.49 Residual compressive strength of geopolymer concrete after exposure to sulfuric acid solution
Figure 4.50 Change in mass of geopolymer mortar cubes exposed to 1% concentration of sulfuric acid solution
Figure 4.51 Residual compressive strength of geopolymer mortar cubes exposed to various concentrations of sulfuric acid solution
LIST OF TABLES
Table 2.1 Applications of Geopolymeric Materials Based on Si:Al Atomic Ratio
Table 3.1 Chemical Composition of Fly Ash (% by mass) 13 Table 3.2 Grading of Combined Aggregates 15 Table 3.3 Concrete Mixture Proportions 16 Table 3.4 Mortar Mixture Proportion 16 Table 3.5 Test Parameters for Creep Test 23 Table 3.6 Test parameters for Drying Shrinkage Test 27 Table 3.7. Test Parameters for Sulfate Resistance Test 29 Table 3.8 Test Parameters of Acid Resistance Test for Geopolymer Concrete
Table 3.9 Test Parameters of Acid Resistance Test for Geopolymer Mortar 33 Table 4.1. Mean compressive strength and unit weight 35 Table 4.2. Compressive strength and sustained stress of creep specimens 39 Table 4.3. Instantaneous Strain and Instantaneous Elastic Modulus 39 Table 4.4. Final specific creep of geopolymer concrete after 1-year loading 47 Table 4.5 Basic creep coefficient (Gilbert 2002) 49 Table 4.6. Heat-cured geopolymer concrete shrinkage specimens 53 Table 4.7 Ratio of compressive strength for different test condition 65
CHAPTER 1: INTRODUCTION
Concrete is one of the most widely used construction materials; it is usually associated with Portland cement as the main component for making concrete. The demand for concrete as a construction material is on the increase. It is estimated that the production of cement will increase from about from 1.5 billion tons in 1995 to 2.2 billion tons in 2010 (Malhotra, 1999).
On the other hand, the climate change due to global warming, one of the greatest environmental issues has become a major concern during the last decade. The global warming is caused by the emission of greenhouse gases, such as CO2, to the atmosphere by human activities. Among the greenhouse gases, CO2 contributes about 65% of global warming (McCaffrey, 2002). The cement industry is responsible for about 6% of all CO2 emissions, because the production of one ton of Portland cement emits approximately one ton of CO2 into the atmosphere (Davidovits, 1994c; McCaffrey, 2002).
Although the use of Portland cement is still unavoidable until the foreseeable future, many efforts are being made in order to reduce the use of Portland cement in concrete. These efforts include the utilisation of supplementary cementing materials such as fly ash, silica fume, granulated blast furnace slag, rice-husk ash and metakaolin, and finding alternative...